#------------------------------------------------------------------------------
#$Date: 2016-03-26 22:56:04 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180523 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/92/7219298.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7219298
loop_
_publ_author_name
'Jiao, Yan-Qing'
'Qin, Chao'
'Zang, Hong-Ying'
'Chen, Wei-Chao'
'Wang, Chun-Gang'
'Zheng, Tian-Tian'
'Shao, Kui-Zhan'
'Su, Zhong-Min'
_publ_section_title
;
 Assembly of organic--inorganic hybrid materials constructed from
 polyoxometalate and metal--1,2,4-triazole units: synthesis, structures,
 magnetic, electrochemical and photocatalytic properties
;
_journal_issue                   10
_journal_name_full               CrystEngComm
_journal_page_first              2176
_journal_paper_doi               10.1039/C4CE02007C
_journal_volume                  17
_journal_year                    2015
_chemical_formula_moiety         'C16 H50 Cl2 Cu6 Ge N24 O55 W12'
_chemical_formula_sum            'C16 H50 Cl2 Cu6 Ge N24 O55 W12'
_chemical_formula_weight         4189.73
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_audit_block_doi                 10.5517/cc13894t
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-01-13 deposited with the CCDC.
2015-01-13 downloaded from the CCDC.
;
_cell_angle_alpha                94.156(5)
_cell_angle_beta                 105.714(5)
_cell_angle_gamma                106.035(5)
_cell_formula_units_Z            1
_cell_length_a                   11.5510(5)
_cell_length_b                   12.1300(5)
_cell_length_c                   14.2860(5)
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.0
_cell_measurement_theta_min      1.5
_cell_volume                     1828.27(15)
_computing_cell_refinement       'SMART (Bruker, 1997)'
_computing_data_collection       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL-PLUS (Sheldrick, 1990)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0504
_diffrn_reflns_av_unetI/netI     0.0973
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            10121
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        24.998
_diffrn_reflns_theta_max         24.998
_diffrn_reflns_theta_min         1.500
_exptl_absorpt_coefficient_mu    21.085
_exptl_absorpt_correction_T_max  0.04
_exptl_absorpt_correction_T_min  0.035
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS(Sheldrick, 1996)'
_exptl_crystal_colour            'dark green'
_exptl_crystal_density_diffrn    3.805
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Block
_exptl_crystal_F_000             1882
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.15
_platon_squeeze_details
;
;
_refine_diff_density_max         5.409
_refine_diff_density_min         -3.209
_refine_diff_density_rms         0.449
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.034
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     511
_refine_ls_number_reflns         6403
_refine_ls_number_restraints     751
_refine_ls_restrained_S_all      1.003
_refine_ls_R_factor_all          0.1178
_refine_ls_R_factor_gt           0.0685
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0904P)²+80.3782P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1697
_refine_ls_wR_factor_ref         0.2041
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4086
_reflns_number_total             6403
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c4ce02007c2.cif
_cod_data_source_block           3
_cod_depositor_comments
'Adding full bibliography for 7219296--7219301.cif.'
_cod_original_cell_volume        1828.27(5)
_cod_database_code               7219298
#BEGIN Tags that were not found in dictionaries:
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
#END Tags that were not found in dictionaries
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
O1 O 0.130(2) 0.701(2) 0.7183(18) 0.073(5) Uani 1 1 d . U .
O2 O 0.099(2) 0.812(2) 1.0298(16) 0.055(3) Uani 1 1 d . U .
O3 O 0.042(4) 0.627(4) 0.955(3) 0.052(2) Uani 0.5 1 d . U P
O4 O -0.104(2) 0.878(2) 0.9254(18) 0.069(6) Uani 1 1 d . U .
O5 O 0.297(4) 0.640(4) 1.052(3) 0.053(2) Uani 0.5 1 d . U P
O5A O 0.370(4) 0.680(4) 1.098(3) 0.054(3) Uani 0.5 1 d . U P
O6 O 0.281(2) 0.566(2) 1.2205(17) 0.060(3) Uani 1 1 d . U .
O7 O 0.102(4) 0.421(4) 0.994(3) 0.054(3) Uani 0.5 1 d . U P
O8 O 0.236(2) 0.322(2) 0.7952(19) 0.066(5) Uani 1 1 d . U .
O9 O -0.062(2) 0.524(2) 0.7379(17) 0.062(3) Uani 1 1 d . U .
O10 O -0.233(2) 0.315(2) 0.6354(17) 0.065(6) Uani 1 1 d . U .
O11 O 0.3622(19) 0.893(2) 1.0856(15) 0.049(3) Uani 1 1 d . U .
O12A O 0.190(4) 0.724(4) 1.156(3) 0.052(3) Uani 0.5 1 d . U P
O12B O 0.258(4) 0.772(4) 1.206(3) 0.051(3) Uani 0.5 1 d . U P
O13 O -0.011(2) 0.328(2) 0.7794(17) 0.061(3) Uani 1 1 d . U .
O14 O 0.027(4) 0.480(4) 0.896(3) 0.053(3) Uani 0.5 1 d . U P
O15 O 0.170(2) 0.521(2) 0.8235(17) 0.061(3) Uani 1 1 d . U .
O16 O 0.4675(19) 0.520(2) 1.1600(17) 0.056(4) Uani 1 1 d . U .
O17 O -0.017(2) 0.721(2) 0.8438(17) 0.062(3) Uani 1 1 d . U .
O18 O 0.217(2) 0.732(2) 0.9204(16) 0.056(2) Uani 1 1 d . U .
O19 O 0.147(4) 0.589(4) 1.086(3) 0.053(3) Uani 0.5 1 d . U P
O20 O 0.108(2) 0.259(2) 0.9325(17) 0.062(3) Uani 1 1 d . U .
O21 O 0.293(2) 0.456(2) 0.9732(17) 0.061(2) Uani 1 1 d . U .
O22 O 0.232(2) 0.349(2) 1.1162(17) 0.061(3) Uani 1 1 d . U .
Ge1 Ge 0.0000 0.5000 1.0000 0.0206(8) Uani 1 2 d S U P
W1 W 0.15779(11) 0.37864(12) 0.85868(9) 0.0391(3) Uani 1 1 d . U .
W2 W 0.31558(12) 0.50807(14) 1.10637(12) 0.0545(4) Uani 1 1 d . U .
W3 W -0.07234(10) 0.76055(10) 0.94955(9) 0.0343(3) Uani 1 1 d . . .
W4 W 0.08812(10) 0.63923(10) 0.80952(7) 0.0321(3) Uani 1 1 d . U .
W5 W 0.24344(11) 0.76689(10) 1.05960(10) 0.0403(4) Uani 1 1 d . U .
W6 W -0.15783(14) 0.37306(12) 0.75043(8) 0.0470(4) Uani 1 1 d . . .
Cu1 Cu 0.5000 1.0000 1.0000 0.0198(9) Uani 1 2 d S . P
Cu2 Cu 0.5323(3) 1.0151(3) 1.2611(2) 0.0305(8) Uani 1 1 d . . .
Cu3 Cu 0.5000 1.0000 1.5000 0.0407(14) Uani 1 2 d S . P
N1 N 0.6501(17) 0.9816(17) 1.1047(13) 0.018(4) Uani 1 1 d . U .
N2 N 0.6604(18) 0.999(2) 1.2006(14) 0.028(5) Uani 1 1 d . . .
N3 N 0.5023(18) 1.145(2) 1.0845(13) 0.028(5) Uani 1 1 d . . .
N4 N 0.520(2) 1.144(2) 1.1856(14) 0.033(6) Uani 1 1 d . . .
N9 N 0.531(2) 1.319(2) 1.1479(18) 0.044(6) Uani 1 1 d . U .
H9 H 0.5366 1.3916 1.1545 0.053 Uiso 1 1 calc R U .
N11 N 0.8430(17) 0.9865(19) 1.1838(13) 0.025(5) Uani 1 1 d . . .
C1 C 0.544(4) 1.253(3) 1.221(2) 0.060(9) Uani 1 1 d . U .
H1 H 0.5662 1.2813 1.2882 0.072 Uiso 1 1 calc R U .
C2 C 0.507(2) 1.247(2) 1.0620(19) 0.029(6) Uani 1 1 d . U .
H2 H 0.4962 1.2676 0.9995 0.035 Uiso 1 1 calc R U .
C3 C 0.775(2) 0.998(3) 1.2461(18) 0.039(8) Uani 1 1 d . . .
H3 H 0.8073 1.0044 1.3141 0.047 Uiso 1 1 calc R U .
C4 C 0.757(3) 0.978(2) 1.0947(17) 0.030(6) Uani 1 1 d . . .
H4 H 0.7733 0.9714 1.0346 0.036 Uiso 1 1 calc R U .
Cl1 Cl 0.6703(8) 1.1489(9) 1.4216(5) 0.060(2) Uani 1 1 d . . .
N8 N 0.3598(17) 0.9978(19) 1.3817(13) 0.024(4) Uani 1 1 d . U .
Cu4 Cu 1.0107(3) 0.9907(4) 1.2244(2) 0.0401(9) Uani 1 1 d . . .
N10 N 0.1785(18) 0.9960(18) 1.2802(13) 0.022(4) Uani 1 1 d . U .
N7 N 0.3799(18) 1.020(2) 1.2959(15) 0.036(6) Uani 1 1 d . . .
C6 C 0.242(2) 0.985(3) 1.3720(19) 0.035(6) Uani 1 1 d . U .
H6 H 0.2048 0.9695 1.4219 0.042 Uiso 1 1 calc R U .
C7 C 0.268(2) 1.015(3) 1.2350(18) 0.030(6) Uani 1 1 d . U .
H7 H 0.2531 1.0246 1.1692 0.036 Uiso 1 1 calc R U .
O1W O 0.695(9) 0.655(8) 1.644(6) 0.32(4) Uani 1 1 d . U .
O2W O 1.0000 1.0000 1.5000 0.17(3) Uani 1 2 d S U P
N5 N 0.5321(18) 0.8745(18) 1.4207(13) 0.022(4) Uani 1 1 d . U .
N6 N 0.540(2) 0.874(3) 1.3286(16) 0.044(7) Uani 1 1 d . . .
C8 C 0.566(4) 0.785(3) 1.301(2) 0.056(10) Uani 1 1 d . . .
H8 H 0.5763 0.7669 1.2399 0.067 Uiso 1 1 calc R U .
N12 N 0.576(3) 0.718(3) 1.375(2) 0.075(9) Uani 1 1 d . U .
H12 H 0.5930 0.6537 1.3774 0.090 Uiso 1 1 calc R U .
C5 C 0.550(3) 0.783(3) 1.445(2) 0.052(8) Uani 1 1 d . U .
H5 H 0.5467 0.7604 1.5053 0.063 Uiso 1 1 calc R U .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
W5 O2 W3 141.1(13) . .
Ge1 O3 W4 124(2) . .
Ge1 O3 W3 122(2) . .
W4 O3 W3 100.7(17) . .
Ge1 O3 W5 113(2) . .
W4 O3 W5 96.4(15) . .
W3 O3 W5 94.4(16) . .
O5A O5 W5 89(5) . .
O5A O5 W2 87(5) . .
W5 O5 W2 146(3) . .
O5 O5A W5 64(4) . .
O5 O5A W2 67(4) . .
W5 O5A W2 122(2) . .
W6 O6 W2 137.8(13) 2_567 .
Ge1 O7 O14 55(2) . .
Ge1 O7 W1 125(2) . .
O14 O7 W1 70(2) . .
Ge1 O7 W3 120(2) . 2_567
O14 O7 W3 138(3) . 2_567
W1 O7 W3 99.6(19) . 2_567
Ge1 O7 W2 114(2) . .
O14 O7 W2 127(3) . .
W1 O7 W2 97.1(16) . .
W3 O7 W2 94.7(16) 2_567 .
W4 O9 W6 138.0(14) . .
W5 O11 Cu1 136.3(11) . .
O12B O12A W5 97(4) . .
O12B O12A O19 138(6) . .
W5 O12A O19 81(2) . .
O12B O12A W6 88(4) . 2_567
W5 O12A W6 156(3) . 2_567
O19 O12A W6 79(2) . 2_567
O12A O12B W5 57(4) . .
O12A O12B W6 66(4) . 2_567
W5 O12B W6 118(2) . 2_567
W1 O13 W6 141.0(14) . .
Ge1 O14 O7 62(2) . .
Ge1 O14 W1 127(3) . .
O7 O14 W1 66(2) . .
Ge1 O14 W4 122(2) . .
O7 O14 W4 136(3) . .
W1 O14 W4 96.5(15) . .
Ge1 O14 W6 117(2) . .
O7 O14 W6 127(3) . .
W1 O14 W6 93.9(16) . .
W4 O14 W6 91.9(15) . .
W1 O15 W4 143.6(13) . .
W3 O17 W4 141.1(15) . .
W4 O18 W5 137.6(12) . .
O12A O19 Ge1 132(3) . .
O12A O19 W5 49.1(18) . .
Ge1 O19 W5 120(2) . .
O12A O19 W6 53.2(19) . 2_567
Ge1 O19 W6 119(2) . 2_567
W5 O19 W6 101.1(17) . 2_567
O12A O19 W2 114(3) . .
Ge1 O19 W2 115(2) . .
W5 O19 W2 99.6(15) . .
W6 O19 W2 98.9(17) 2_567 .
W3 O20 W1 140.7(15) 2_567 .
W2 O21 W1 138.1(13) . .
W3 O22 W2 134.6(13) 2_567 .
O14 Ge1 O14 180.00(2) . 2_567
O14 Ge1 O3 112(2) . 2_567
O14 Ge1 O3 68(2) 2_567 2_567
O14 Ge1 O3 68(2) . .
O14 Ge1 O3 112(2) 2_567 .
O3 Ge1 O3 179.999(13) 2_567 .
O14 Ge1 O7 63(2) . .
O14 Ge1 O7 117(2) 2_567 .
O3 Ge1 O7 69(2) 2_567 .
O3 Ge1 O7 111(2) . .
O14 Ge1 O7 117(2) . 2_567
O14 Ge1 O7 63(2) 2_567 2_567
O3 Ge1 O7 111(2) 2_567 2_567
O3 Ge1 O7 69(2) . 2_567
O7 Ge1 O7 180(3) . 2_567
O14 Ge1 O19 74(2) . 2_567
O14 Ge1 O19 106(2) 2_567 2_567
O3 Ge1 O19 74(2) 2_567 2_567
O3 Ge1 O19 106(2) . 2_567
O7 Ge1 O19 103(2) . 2_567
O7 Ge1 O19 77(2) 2_567 2_567
O14 Ge1 O19 106(2) . .
O14 Ge1 O19 74(2) 2_567 .
O3 Ge1 O19 106(2) 2_567 .
O3 Ge1 O19 74(2) . .
O7 Ge1 O19 77(2) . .
O7 Ge1 O19 103(2) 2_567 .
O19 Ge1 O19 180.0 2_567 .
O8 W1 O15 104.5(12) . .
O8 W1 O13 105.1(12) . .
O15 W1 O13 88.6(10) . .
O8 W1 O21 99.7(12) . .
O15 W1 O21 86.5(10) . .
O13 W1 O21 155.2(11) . .
O8 W1 O20 102.3(12) . .
O15 W1 O20 153.1(11) . .
O13 W1 O20 85.9(10) . .
O21 W1 O20 87.6(10) . .
O8 W1 O7 155.1(15) . .
O15 W1 O7 93.7(14) . .
O13 W1 O7 92.0(13) . .
O21 W1 O7 64.1(13) . .
O20 W1 O7 60.3(14) . .
O8 W1 O14 160.2(15) . .
O15 W1 O14 60.7(13) . .
O13 W1 O14 63.9(13) . .
O21 W1 O14 92.7(13) . .
O20 W1 O14 93.5(14) . .
O7 W1 O14 44.6(16) . .
O16 W2 O5 112.2(16) . .
O16 W2 O21 102.4(11) . .
O5 W2 O21 79.9(16) . .
O16 W2 O6 97.6(11) . .
O5 W2 O6 89.6(16) . .
O21 W2 O6 159.7(10) . .
O16 W2 O22 101.4(11) . .
O5 W2 O22 145.9(16) . .
O21 W2 O22 87.6(10) . .
O6 W2 O22 91.7(10) . .
O16 W2 O5A 88.8(16) . .
O5 W2 O5A 26.1(15) . .
O21 W2 O5A 96.0(15) . .
O6 W2 O5A 81.0(15) . .
O22 W2 O5A 168.3(15) . .
O16 W2 O19 149.2(13) . .
O5 W2 O19 51.0(17) . .
O21 W2 O19 99.4(13) . .
O6 W2 O19 60.9(13) . .
O22 W2 O19 101.1(13) . .
O5A W2 O19 67.4(17) . .
O16 W2 O7 156.7(14) . .
O5 W2 O7 82.0(18) . .
O21 W2 O7 60.5(13) . .
O6 W2 O7 101.1(13) . .
O22 W2 O7 64.3(13) . .
O5A W2 O7 107.8(18) . .
O19 W2 O7 54.1(16) . .
O4 W3 O20 103.4(13) . 2_567
O4 W3 O17 102.1(12) . .
O20 W3 O17 154.4(12) 2_567 .
O4 W3 O22 99.5(12) . 2_567
O20 W3 O22 88.4(10) 2_567 2_567
O17 W3 O22 88.4(10) . 2_567
O4 W3 O2 104.1(11) . .
O20 W3 O2 84.4(10) 2_567 .
O17 W3 O2 88.4(10) . .
O22 W3 O2 156.3(11) 2_567 .
O4 W3 O3 155.0(14) . .
O20 W3 O3 96.8(14) 2_567 .
O17 W3 O3 58.3(13) . .
O22 W3 O3 95.5(13) 2_567 .
O2 W3 O3 63.1(12) . .
O4 W3 O7 155.9(15) . 2_567
O20 W3 O7 58.7(14) 2_567 2_567
O17 W3 O7 97.0(14) . 2_567
O22 W3 O7 66.4(13) 2_567 2_567
O2 W3 O7 90.8(13) . 2_567
O3 W3 O7 49.0(15) . 2_567
O1 W4 O9 100.4(11) . .
O1 W4 O18 101.4(11) . .
O9 W4 O18 158.1(10) . .
O1 W4 O17 104.5(13) . .
O9 W4 O17 86.2(11) . .
O18 W4 O17 86.4(10) . .
O1 W4 O15 102.9(13) . .
O9 W4 O15 88.1(10) . .
O18 W4 O15 89.0(10) . .
O17 W4 O15 152.6(10) . .
O1 W4 O3 158.2(16) . .
O9 W4 O3 93.2(13) . .
O18 W4 O3 65.3(12) . .
O17 W4 O3 59.2(14) . .
O15 W4 O3 94.4(14) . .
O1 W4 O14 155.3(15) . .
O9 W4 O14 66.1(13) . .
O18 W4 O14 94.2(12) . .
O17 W4 O14 95.4(14) . .
O15 W4 O14 58.0(13) . .
O3 W4 O14 46.5(16) . .
O11 W5 O12A 115.9(17) . .
O11 W5 O5 112.8(16) . .
O12A W5 O5 90(2) . .
O11 W5 O2 103.9(11) . .
O12A W5 O2 81.1(17) . .
O5 W5 O2 142.3(16) . .
O11 W5 O18 99.1(10) . .
O12A W5 O18 144.9(17) . .
O5 W5 O18 78.0(16) . .
O2 W5 O18 88.2(10) . .
O11 W5 O5A 90.0(15) . .
O12A W5 O5A 88(2) . .
O5 W5 O5A 26.5(16) . .
O2 W5 O5A 165.2(15) . .
O18 W5 O5A 94.7(15) . .
O11 W5 O12B 90.3(14) . .
O12A W5 O12B 26.5(16) . .
O5 W5 O12B 94(2) . .
O2 W5 O12B 93.6(15) . .
O18 W5 O12B 169.7(15) . .
O5A W5 O12B 81.0(19) . .
O11 W5 O19 154.0(13) . .
O12A W5 O19 49.4(19) . .
O5 W5 O19 53.8(18) . .
O2 W5 O19 95.1(14) . .
O18 W5 O19 99.0(13) . .
O5A W5 O19 70.1(17) . .
O12B W5 O19 70.7(17) . .
O11 W5 O3 153.1(13) . .
O12A W5 O3 85.1(19) . .
O5 W5 O3 81.9(19) . .
O2 W5 O3 60.9(13) . .
O18 W5 O3 60.7(12) . .
O5A W5 O3 108.0(18) . .
O12B W5 O3 111.6(16) . .
O19 W5 O3 52.7(16) . .
O10 W6 O13 104.1(12) . .
O10 W6 O12A 115.4(17) . 2_567
O13 W6 O12A 80.5(16) . 2_567
O10 W6 O6 99.3(12) . 2_567
O13 W6 O6 155.9(10) . 2_567
O12A W6 O6 84.5(16) 2_567 2_567
O10 W6 O9 101.8(11) . .
O13 W6 O9 89.8(11) . .
O12A W6 O9 142.8(16) 2_567 .
O6 W6 O9 90.9(11) 2_567 .
O10 W6 O12B 89.7(16) . 2_567
O13 W6 O12B 92.3(15) . 2_567
O12A W6 O12B 26.4(15) 2_567 2_567
O6 W6 O12B 82.1(15) 2_567 2_567
O9 W6 O12B 167.4(15) . 2_567
O10 W6 O19 152.9(14) . 2_567
O13 W6 O19 93.9(14) . 2_567
O12A W6 O19 47.4(18) 2_567 2_567
O6 W6 O19 62.2(13) 2_567 2_567
O9 W6 O19 98.3(13) . 2_567
O12B W6 O19 69.2(17) 2_567 2_567
O10 W6 O14 156.9(14) . .
O13 W6 O14 60.2(13) . .
O12A W6 O14 80.5(17) 2_567 .
O6 W6 O14 98.9(13) 2_567 .
O9 W6 O14 63.7(12) . .
O12B W6 O14 106.9(16) 2_567 .
O19 W6 O14 50.2(14) 2_567 .
N1 Cu1 N1 180.0 . 2_677
N1 Cu1 N3 91.8(8) . .
N1 Cu1 N3 88.2(8) 2_677 .
N1 Cu1 N3 88.2(8) . 2_677
N1 Cu1 N3 91.8(8) 2_677 2_677
N3 Cu1 N3 180.0 . 2_677
N1 Cu1 O11 91.3(7) . 2_677
N1 Cu1 O11 88.7(7) 2_677 2_677
N3 Cu1 O11 94.6(8) . 2_677
N3 Cu1 O11 85.4(8) 2_677 2_677
N1 Cu1 O11 88.7(7) . .
N1 Cu1 O11 91.3(7) 2_677 .
N3 Cu1 O11 85.4(8) . .
N3 Cu1 O11 94.6(8) 2_677 .
O11 Cu1 O11 180.0(8) 2_677 .
N2 Cu2 N7 168.8(8) . .
N2 Cu2 N4 86.5(10) . .
N7 Cu2 N4 89.4(10) . .
N2 Cu2 N6 91.8(9) . .
N7 Cu2 N6 91.5(10) . .
N4 Cu2 N6 175.6(9) . .
N2 Cu2 Cl1 100.8(6) . .
N7 Cu2 Cl1 89.9(7) . .
N4 Cu2 Cl1 94.2(7) . .
N6 Cu2 Cl1 90.1(7) . .
N8 Cu3 N8 180.0(11) . 2_678
N8 Cu3 N5 92.3(8) . 2_678
N8 Cu3 N5 87.7(8) 2_678 2_678
N8 Cu3 N5 87.7(8) . .
N8 Cu3 N5 92.3(8) 2_678 .
N5 Cu3 N5 180.000(11) 2_678 .
C4 N1 N2 109.3(19) . .
C4 N1 Cu1 127.5(16) . .
N2 N1 Cu1 121.6(15) . .
C3 N2 N1 104.8(19) . .
C3 N2 Cu2 127.0(17) . .
N1 N2 Cu2 128.2(15) . .
C2 N3 N4 112(2) . .
C2 N3 Cu1 129.2(17) . .
N4 N3 Cu1 118.5(18) . .
C1 N4 N3 104(2) . .
C1 N4 Cu2 127(2) . .
N3 N4 Cu2 128.8(18) . .
C2 N9 C1 106(3) . .
C2 N9 H9 126.8 . .
C1 N9 H9 126.8 . .
C3 N11 C4 101.4(19) . .
C3 N11 Cu4 124.0(16) . .
C4 N11 Cu4 134.5(16) . .
N4 C1 N9 111(3) . .
N4 C1 H1 124.4 . .
N9 C1 H1 124.4 . .
N3 C2 N9 107(2) . .
N3 C2 H2 126.6 . .
N9 C2 H2 126.6 . .
N2 C3 N11 113(2) . .
N2 C3 H3 123.4 . .
N11 C3 H3 123.4 . .
N1 C4 N11 111(2) . .
N1 C4 H4 124.4 . .
N11 C4 H4 124.4 . .
C6 N8 N7 107.8(19) . .
C6 N8 Cu3 130.1(17) . .
N7 N8 Cu3 121.9(14) . .
N11 Cu4 N10 173.3(8) . 1_655
C7 N10 C6 103(2) . .
C7 N10 Cu4 125.8(16) . 1_455
C6 N10 Cu4 131.3(18) . 1_455
C7 N7 N8 105.7(19) . .
C7 N7 Cu2 127.7(17) . .
N8 N7 Cu2 124.4(16) . .
N8 C6 N10 112(2) . .
N8 C6 H6 124.1 . .
N10 C6 H6 124.1 . .
N10 C7 N7 112(2) . .
N10 C7 H7 124.1 . .
N7 C7 H7 124.1 . .
C5 N5 N6 106(3) . .
C5 N5 Cu3 129(2) . .
N6 N5 Cu3 125.9(19) . .
C8 N6 N5 110(3) . .
C8 N6 Cu2 129.0(19) . .
N5 N6 Cu2 120(2) . .
N6 C8 N12 109(3) . .
N6 C8 H8 125.4 . .
N12 C8 H8 125.4 . .
C5 N12 C8 101(3) . .
C5 N12 H12 129.6 . .
C8 N12 H12 129.6 . .
N5 C5 N12 114(3) . .
N5 C5 H5 122.9 . .
N12 C5 H5 122.9 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
O1 W4 1.67(2) .
O2 W5 1.85(2) .
O2 W3 1.90(2) .
O3 Ge1 1.71(4) .
O3 W4 2.28(4) .
O3 W3 2.35(5) .
O3 W5 2.47(4) .
O4 W3 1.61(3) .
O5 O5A 0.90(5) .
O5 W5 1.81(5) .
O5 W2 1.88(5) .
O5A W5 2.01(5) .
O5A W2 2.03(5) .
O6 W6 1.90(3) 2_567
O6 W2 1.91(2) .
O7 Ge1 1.73(5) .
O7 O14 1.75(6) .
O7 W1 2.27(5) .
O7 W3 2.37(5) 2_567
O7 W2 2.44(4) .
O8 W1 1.67(2) .
O9 W4 1.87(2) .
O9 W6 1.91(2) .
O10 W6 1.63(2) .
O11 W5 1.68(2) .
O11 Cu1 2.42(2) .
O12A O12B 0.92(5) .
O12A W5 1.72(4) .
O12A O19 1.73(6) .
O12A W6 1.88(4) 2_567
O12B W5 2.04(4) .
O12B W6 2.06(4) 2_567
O13 W1 1.87(2) .
O13 W6 1.88(3) .
O14 Ge1 1.61(4) .
O14 W1 2.34(5) .
O14 W4 2.41(4) .
O14 W6 2.50(4) .
O15 W1 1.81(3) .
O15 W4 1.92(3) .
O16 W2 1.68(2) .
O17 W3 1.87(2) .
O17 W4 1.91(3) .
O18 W4 1.88(2) .
O18 W5 1.92(2) .
O19 Ge1 1.80(4) .
O19 W5 2.25(4) .
O19 W6 2.31(4) 2_567
O19 W2 2.37(5) .
O20 W3 1.85(2) 2_567
O20 W1 1.91(2) .
O21 W2 1.88(2) .
O21 W1 1.89(2) .
O22 W3 1.89(2) 2_567
O22 W2 1.94(2) .
Ge1 O14 1.61(4) 2_567
Ge1 O3 1.71(4) 2_567
Ge1 O7 1.73(5) 2_567
Ge1 O19 1.80(4) 2_567
W3 O20 1.85(2) 2_567
W3 O22 1.89(2) 2_567
W3 O7 2.37(5) 2_567
W6 O12A 1.88(4) 2_567
W6 O6 1.90(3) 2_567
W6 O12B 2.06(4) 2_567
W6 O19 2.31(4) 2_567
Cu1 N1 2.037(18) .
Cu1 N1 2.037(18) 2_677
Cu1 N3 2.05(2) .
Cu1 N3 2.05(2) 2_677
Cu1 O11 2.42(2) 2_677
Cu2 N2 1.951(19) .
Cu2 N7 1.97(2) .
Cu2 N4 1.98(2) .
Cu2 N6 2.03(3) .
Cu2 Cl1 2.547(9) .
Cu3 N8 1.992(17) .
Cu3 N8 1.992(17) 2_678
Cu3 N5 2.01(2) 2_678
Cu3 N5 2.01(2) .
N1 C4 1.29(3) .
N1 N2 1.34(3) .
N2 C3 1.31(3) .
N3 C2 1.29(3) .
N3 N4 1.41(3) .
N4 C1 1.30(4) .
N9 C2 1.37(3) .
N9 C1 1.37(4) .
N9 H9 0.8600 .
N11 C3 1.35(3) .
N11 C4 1.36(3) .
N11 Cu4 1.850(19) .
C1 H1 0.9300 .
C2 H2 0.9300 .
C3 H3 0.9300 .
C4 H4 0.9300 .
N8 C6 1.30(3) .
N8 N7 1.34(3) .
Cu4 N10 1.867(19) 1_655
N10 C7 1.33(3) .
N10 C6 1.35(3) .
N10 Cu4 1.867(18) 1_455
N7 C7 1.34(3) .
C6 H6 0.9300 .
C7 H7 0.9300 .
N5 C5 1.24(4) .
N5 N6 1.34(3) .
N6 C8 1.27(4) .
C8 N12 1.38(4) .
C8 H8 0.9300 .
N12 C5 1.37(5) .
N12 H12 0.8600 .
C5 H5 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
W2 O5 O5A W5 -146(2) . .
W5 O5 O5A W2 146(2) . .
O19 O12A O12B W5 85(7) . .
W6 O12A O12B W5 156(3) 2_567 .
W5 O12A O12B W6 -156(3) . 2_567
O19 O12A O12B W6 -71(7) . 2_567
W1 O7 O14 Ge1 179.8(19) . .
W3 O7 O14 Ge1 98(4) 2_567 .
W2 O7 O14 Ge1 -96(3) . .
Ge1 O7 O14 W1 -180(2) . .
W3 O7 O14 W1 -82(4) 2_567 .
W2 O7 O14 W1 84(3) . .
Ge1 O7 O14 W4 107(4) . .
W1 O7 O14 W4 -73(4) . .
W3 O7 O14 W4 -155(3) 2_567 .
W2 O7 O14 W4 11(6) . .
Ge1 O7 O14 W6 -104(3) . .
W1 O7 O14 W6 75(3) . .
W3 O7 O14 W6 -6(6) 2_567 .
W2 O7 O14 W6 159(2) . .
O12B O12A O19 Ge1 172(7) . .
W5 O12A O19 Ge1 -97(4) . .
W6 O12A O19 Ge1 98(4) 2_567 .
O12B O12A O19 W5 -91(8) . .
W6 O12A O19 W5 -165(2) 2_567 .
O12B O12A O19 W6 75(8) . 2_567
W5 O12A O19 W6 165(2) . 2_567
O12B O12A O19 W2 -9(9) . .
W5 O12A O19 W2 82(2) . .
W6 O12A O19 W2 -83(2) 2_567 .
O7 O14 Ge1 O3 -51(3) . 2_567
W1 O14 Ge1 O3 -50(3) . 2_567
W4 O14 Ge1 O3 -180(2) . 2_567
W6 O14 Ge1 O3 69(3) . 2_567
O7 O14 Ge1 O3 129(3) . .
W1 O14 Ge1 O3 130(3) . .
W4 O14 Ge1 O3 0(2) . .
W6 O14 Ge1 O3 -111(3) . .
W1 O14 Ge1 O7 0(2) . .
W4 O14 Ge1 O7 -129(3) . .
W6 O14 Ge1 O7 119(3) . .
O7 O14 Ge1 O7 180.00(5) . 2_567
W1 O14 Ge1 O7 -180(2) . 2_567
W4 O14 Ge1 O7 51(3) . 2_567
W6 O14 Ge1 O7 -61(3) . 2_567
O7 O14 Ge1 O19 -115(3) . 2_567
W1 O14 Ge1 O19 -115(3) . 2_567
W4 O14 Ge1 O19 116(3) . 2_567
W6 O14 Ge1 O19 5(2) . 2_567
O7 O14 Ge1 O19 65(3) . .
W1 O14 Ge1 O19 65(3) . .
W4 O14 Ge1 O19 -64(3) . .
W6 O14 Ge1 O19 -175(2) . .
W4 O3 Ge1 O14 0(2) . .
W3 O3 Ge1 O14 133(3) . .
W5 O3 Ge1 O14 -116(3) . .
W4 O3 Ge1 O14 180(2) . 2_567
W3 O3 Ge1 O14 -47(3) . 2_567
W5 O3 Ge1 O14 64(3) . 2_567
W4 O3 Ge1 O7 47(3) . .
W3 O3 Ge1 O7 -180(2) . .
W5 O3 Ge1 O7 -68(3) . .
W4 O3 Ge1 O7 -133(3) . 2_567
W3 O3 Ge1 O7 0(2) . 2_567
W5 O3 Ge1 O7 112(3) . 2_567
W4 O3 Ge1 O19 -64(3) . 2_567
W3 O3 Ge1 O19 69(3) . 2_567
W5 O3 Ge1 O19 -180(2) . 2_567
W4 O3 Ge1 O19 116(3) . .
W3 O3 Ge1 O19 -111(3) . .
W5 O3 Ge1 O19 0(2) . .
W1 O7 Ge1 O14 0(2) . .
W3 O7 Ge1 O14 -130(3) 2_567 .
W2 O7 Ge1 O14 119(3) . .
O14 O7 Ge1 O14 180.00(5) . 2_567
W1 O7 Ge1 O14 180(2) . 2_567
W3 O7 Ge1 O14 50(3) 2_567 2_567
W2 O7 Ge1 O14 -61(3) . 2_567
O14 O7 Ge1 O3 130(3) . 2_567
W1 O7 Ge1 O3 130(3) . 2_567
W3 O7 Ge1 O3 0(2) 2_567 2_567
W2 O7 Ge1 O3 -111(3) . 2_567
O14 O7 Ge1 O3 -50(3) . .
W1 O7 Ge1 O3 -50(3) . .
W3 O7 Ge1 O3 -180(2) 2_567 .
W2 O7 Ge1 O3 69(3) . .
O14 O7 Ge1 O19 63(2) . 2_567
W1 O7 Ge1 O19 63(3) . 2_567
W3 O7 Ge1 O19 -66(3) 2_567 2_567
W2 O7 Ge1 O19 -178(2) . 2_567
O14 O7 Ge1 O19 -117(2) . .
W1 O7 Ge1 O19 -117(3) . .
W3 O7 Ge1 O19 114(3) 2_567 .
W2 O7 Ge1 O19 2(2) . .
O12A O19 Ge1 O14 120(4) . .
W5 O19 Ge1 O14 60(3) . .
W6 O19 Ge1 O14 -175(2) 2_567 .
W2 O19 Ge1 O14 -59(3) . .
O12A O19 Ge1 O14 -60(4) . 2_567
W5 O19 Ge1 O14 -120(3) . 2_567
W6 O19 Ge1 O14 5(3) 2_567 2_567
W2 O19 Ge1 O14 121(3) . 2_567
O12A O19 Ge1 O3 -120(4) . 2_567
W5 O19 Ge1 O3 180(2) . 2_567
W6 O19 Ge1 O3 -55(3) 2_567 2_567
W2 O19 Ge1 O3 61(3) . 2_567
O12A O19 Ge1 O3 60(4) . .
W5 O19 Ge1 O3 0(2) . .
W6 O19 Ge1 O3 125(3) 2_567 .
W2 O19 Ge1 O3 -119(3) . .
O12A O19 Ge1 O7 177(4) . .
W5 O19 Ge1 O7 116(3) . .
W6 O19 Ge1 O7 -119(3) 2_567 .
W2 O19 Ge1 O7 -2(2) . .
O12A O19 Ge1 O7 -3(4) . 2_567
W5 O19 Ge1 O7 -64(3) . 2_567
W6 O19 Ge1 O7 61(3) 2_567 2_567
W2 O19 Ge1 O7 178(2) . 2_567
W4 O15 W1 O8 153(2) . .
W4 O15 W1 O13 48(2) . .
W4 O15 W1 O21 -108(2) . .
W4 O15 W1 O20 -30(4) . .
W4 O15 W1 O7 -44(2) . .
W4 O15 W1 O14 -13(2) . .
W6 O13 W1 O8 -150(2) . .
W6 O13 W1 O15 -45(2) . .
W6 O13 W1 O21 33(4) . .
W6 O13 W1 O20 108(2) . .
W6 O13 W1 O7 48(2) . .
W6 O13 W1 O14 12(2) . .
W2 O21 W1 O8 -156(2) . .
W2 O21 W1 O15 100(2) . .
W2 O21 W1 O13 21(4) . .
W2 O21 W1 O20 -54(2) . .
W2 O21 W1 O7 4(2) . .
W2 O21 W1 O14 39(2) . .
O5A O5 W2 O16 -28(5) . .
W5 O5 W2 O16 -111(5) . .
O5A O5 W2 O21 -127(4) . .
W5 O5 W2 O21 150(5) . .
O5A O5 W2 O6 70(4) . .
W5 O5 W2 O6 -13(5) . .
O5A O5 W2 O22 163(3) . .
W5 O5 W2 O22 79(6) . .
W5 O5 W2 O5A -83(6) . .
O5A O5 W2 O19 122(5) . .
W5 O5 W2 O19 39(4) . .
O5A O5 W2 O7 171(5) . .
W5 O5 W2 O7 88(5) . .
W1 O21 W2 O16 159(2) . .
W1 O21 W2 O5 -90(2) . .
W1 O21 W2 O6 -30(4) . .
W1 O21 W2 O22 58(2) . .
W1 O21 W2 O5A -111(2) . .
W1 O21 W2 O19 -43(2) . .
W1 O21 W2 O7 -4(2) . .
W4 O17 W3 O4 154(2) . .
W4 O17 W3 O20 -24(4) . 2_567
W4 O17 W3 O22 -107(2) . 2_567
W4 O17 W3 O2 50(2) . .
W4 O17 W3 O3 -9.4(19) . .
W4 O17 W3 O7 -41(2) . 2_567
W6 O9 W4 O1 151(2) . .
W6 O9 W4 O18 -34(4) . .
W6 O9 W4 O17 -105(2) . .
W6 O9 W4 O15 49(2) . .
W6 O9 W4 O3 -46(2) . .
W6 O9 W4 O14 -7(2) . .
W5 O18 W4 O1 161(2) . .
W5 O18 W4 O9 -14(4) . .
W5 O18 W4 O17 57(2) . .
W5 O18 W4 O15 -96(2) . .
W5 O18 W4 O3 -1(2) . .
W5 O18 W4 O14 -39(2) . .
Cu1 O11 W5 O12A 173(2) . .
Cu1 O11 W5 O5 70(2) . .
Cu1 O11 W5 O2 -100.8(17) . .
Cu1 O11 W5 O18 -10.4(19) . .
Cu1 O11 W5 O5A 84(2) . .
Cu1 O11 W5 O12B 165(2) . .
Cu1 O11 W5 O19 123(3) . .
Cu1 O11 W5 O3 -49(4) . .
O12B O12A W5 O11 -16(5) . .
O19 O12A W5 O11 -154.2(19) . .
W6 O12A W5 O11 -116(7) 2_567 .
O12B O12A W5 O5 100(5) . .
O19 O12A W5 O5 -39(3) . .
W6 O12A W5 O5 -1(7) 2_567 .
O12B O12A W5 O2 -117(5) . .
O19 O12A W5 O2 105(2) . .
W6 O12A W5 O2 143(7) 2_567 .
O12B O12A W5 O18 169(4) . .
O19 O12A W5 O18 31(4) . .
W6 O12A W5 O18 69(8) 2_567 .
O12B O12A W5 O5A 73(5) . .
O19 O12A W5 O5A -65(2) . .
W6 O12A W5 O5A -27(7) 2_567 .
O19 O12A W5 O12B -138(6) . .
W6 O12A W5 O12B -100(9) 2_567 .
O12B O12A W5 O19 138(6) . .
W6 O12A W5 O19 38(6) 2_567 .
O12B O12A W5 O3 -179(5) . .
O19 O12A W5 O3 43(2) . .
W6 O12A W5 O3 81(7) 2_567 .
O5A O5 W5 O11 33(5) . .
W2 O5 W5 O11 115(5) . .
O5A O5 W5 O12A -86(4) . .
W2 O5 W5 O12A -3(5) . .
O5A O5 W5 O2 -161(3) . .
W2 O5 W5 O2 -79(6) . .
O5A O5 W5 O18 128(4) . .
W2 O5 W5 O18 -150(5) . .
W2 O5 W5 O5A 82(6) . .
O5A O5 W5 O12B -59(4) . .
W2 O5 W5 O12B 23(5) . .
O5A O5 W5 O19 -122(5) . .
W2 O5 W5 O19 -39(4) . .
O5A O5 W5 O3 -171(4) . .
W2 O5 W5 O3 -88(5) . .
W3 O2 W5 O11 148(2) . .
W3 O2 W5 O12A -97(3) . .
W3 O2 W5 O5 -18(4) . .
W3 O2 W5 O18 49(2) . .
W3 O2 W5 O5A -52(7) . .
W3 O2 W5 O12B -120(2) . .
W3 O2 W5 O19 -49(2) . .
W3 O2 W5 O3 -7.6(19) . .
W1 O13 W6 O10 150(2) . .
W1 O13 W6 O12A -96(3) . 2_567
W1 O13 W6 O6 -44(4) . 2_567
W1 O13 W6 O9 48(2) . .
W1 O13 W6 O12B -120(2) . 2_567
W1 O13 W6 O19 -51(2) . 2_567
W1 O13 W6 O14 -12(2) . .
C4 N1 N2 C3 -4(3) . .
Cu1 N1 N2 C3 -170(2) . .
C4 N1 N2 Cu2 178(2) . .
Cu1 N1 N2 Cu2 12(3) . .
C2 N3 N4 C1 -4(3) . .
Cu1 N3 N4 C1 167(2) . .
C2 N3 N4 Cu2 -175.6(18) . .
Cu1 N3 N4 Cu2 -4(3) . .
N3 N4 C1 N9 6(3) . .
Cu2 N4 C1 N9 177.0(19) . .
C2 N9 C1 N4 -5(4) . .
N4 N3 C2 N9 1(3) . .
Cu1 N3 C2 N9 -168.7(16) . .
C1 N9 C2 N3 2(3) . .
N1 N2 C3 N11 3(3) . .
Cu2 N2 C3 N11 -179.1(19) . .
C4 N11 C3 N2 -1(3) . .
Cu4 N11 C3 N2 176(2) . .
N2 N1 C4 N11 3(3) . .
Cu1 N1 C4 N11 168.9(17) . .
C3 N11 C4 N1 -2(3) . .
Cu4 N11 C4 N1 -178(2) . .
C6 N8 N7 C7 -2(3) . .
Cu3 N8 N7 C7 -177.8(19) . .
C6 N8 N7 Cu2 -167(2) . .
Cu3 N8 N7 Cu2 18(3) . .
N7 N8 C6 N10 1(3) . .
Cu3 N8 C6 N10 176.0(18) . .
C7 N10 C6 N8 1(3) . .
Cu4 N10 C6 N8 -177.9(19) 1_455 .
C6 N10 C7 N7 -2(3) . .
Cu4 N10 C7 N7 176.6(19) 1_455 .
N8 N7 C7 N10 3(3) . .
Cu2 N7 C7 N10 166.5(19) . .
C5 N5 N6 C8 -2(3) . .
Cu3 N5 N6 C8 177(2) . .
C5 N5 N6 Cu2 -174(2) . .
Cu3 N5 N6 Cu2 5(3) . .
N5 N6 C8 N12 1(4) . .
Cu2 N6 C8 N12 172(2) . .
N6 C8 N12 C5 1(4) . .
N6 N5 C5 N12 2(4) . .
Cu3 N5 C5 N12 -177(2) . .
C8 N12 C5 N5 -2(4) . .
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.010 0.500 0.500 283 216 ' '
